#------------------------------------------------------------------------------
#$Date: 2021-04-09 11:07:55 +0300 (Fri, 09 Apr 2021) $
#$Revision: 264009 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/16/1561600.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561600
loop_
_publ_author_name
'Wang, Mo'
'Sun, Wenlong'
'Pang, Haijun'
'Ma, Huiyuan'
'Yu, Jia'
'Zhang, Zhuanfang'
'Niu, Ying'
'Yin, Mingming'
_publ_section_title
;
 Tuning the microstructures of decavanadate-based supramolecular hybrids
 via regularly changing the spacers of bis(triazole) ligands
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              175
_journal_page_last               182
_journal_paper_doi               10.1016/j.jssc.2015.12.033
_journal_volume                  235
_journal_year                    2016
_chemical_formula_sum            'C16 H56 N12 O44 V10 Zn3'
_chemical_formula_weight         1826.31
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                94.944(5)
_cell_angle_beta                 111.881(5)
_cell_angle_gamma                107.708(5)
_cell_formula_units_Z            1
_cell_length_a                   10.838(5)
_cell_length_b                   11.934(5)
_cell_length_c                   12.293(5)
_cell_measurement_reflns_used    4007
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.30
_cell_measurement_theta_min      2.17
_cell_volume                     1369.3(10)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0183
_diffrn_reflns_av_sigmaI/netI    0.0366
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7216
_diffrn_reflns_theta_full        25.25
_diffrn_reflns_theta_max         25.25
_diffrn_reflns_theta_min         2.17
_exptl_absorpt_coefficient_mu    3.027
_exptl_absorpt_correction_T_max  0.546
_exptl_absorpt_correction_T_min  0.474
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2003)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             876
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.20
_refine_diff_density_max         2.080
_refine_diff_density_min         -0.785
_refine_diff_density_rms         0.136
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     385
_refine_ls_number_reflns         4894
_refine_ls_number_restraints     40
_refine_ls_restrained_S_all      1.153
_refine_ls_R_factor_all          0.0478
_refine_ls_R_factor_gt           0.0414
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1444
_refine_ls_wR_factor_ref         0.1491
_reflns_number_gt                4243
_reflns_number_total             4967
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2016-235-175.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_refine_ls_hydrogen_treatment' value 'Refall' was changed
to 'refall' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      'P-1   '
_cod_database_code               1561600
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn -0.30517(5) -0.13061(5) -0.41227(5) 0.01739(18) Uani 1 1 d . . .
Zn2 Zn 0.0000 -0.5000 0.0000 0.0304(2) Uani 1 2 d S . .
V1 V -0.90994(7) -0.51280(6) -0.57817(6) 0.0105(2) Uani 1 1 d . . .
V2 V -0.83691(8) -0.25265(7) -0.26418(7) 0.0155(2) Uani 1 1 d . . .
V3 V -0.67359(8) -0.27810(7) -0.41436(7) 0.0132(2) Uani 1 1 d . . .
V4 V -0.97797(8) -0.27556(6) -0.54334(7) 0.0130(2) Uani 1 1 d . . .
V5 V -0.77268(8) -0.48962(7) -0.29750(6) 0.0132(2) Uani 1 1 d . . .
O1 O -0.7727(3) -0.3683(3) -0.1943(3) 0.0148(7) Uani 1 1 d . . .
O2 O -0.6734(3) -0.1894(3) -0.2883(3) 0.0166(7) Uani 1 1 d . . .
O1W O 0.1841(5) -0.3791(4) 0.0018(4) 0.0486(12) Uani 1 1 d . . .
O3 O -0.6991(4) -0.5635(3) -0.2091(3) 0.0250(8) Uani 1 1 d . . .
O2W O 0.0219(5) -0.3768(4) 0.1417(3) 0.0435(11) Uani 1 1 d . . .
O4 O -0.8905(3) -0.3974(3) -0.4325(3) 0.0112(6) Uani 1 1 d . . .
O3W O 0.5853(5) -0.4699(4) -0.3277(5) 0.0509(12) Uani 1 1 d . . .
O5 O -1.0206(3) -0.4226(3) -0.6642(3) 0.0114(6) Uani 1 1 d . . .
O4W O -0.1654(5) 0.1465(4) -0.1181(4) 0.0446(11) Uani 1 1 d . . .
O6 O -1.0475(3) -0.1969(3) -0.6306(3) 0.0225(8) Uani 1 1 d . . .
O5W O -0.1259(5) -0.4184(4) -0.1244(4) 0.0430(10) Uani 1 1 d . . .
O7 O -0.9690(3) -0.6288(3) -0.6993(3) 0.0151(7) Uani 1 1 d . . .
O6W O -0.2973(4) 0.0441(3) -0.3624(3) 0.0280(8) Uani 1 1 d . . .
O8 O -0.8489(3) -0.6017(3) -0.4578(3) 0.0125(6) Uani 1 1 d . . .
O7W O -0.0946(4) -0.0573(3) -0.3989(4) 0.0342(9) Uani 1 1 d . . .
O9 O -0.7942(3) -0.2195(3) -0.5268(3) 0.0148(6) Uani 1 1 d . . .
O8W O -0.3255(4) -0.3164(3) -0.4671(3) 0.0288(8) Uani 1 1 d . . .
O10 O -0.5212(3) -0.2082(3) -0.4159(3) 0.0193(7) Uani 1 1 d . . .
O11 O -0.8114(4) -0.1591(3) -0.1488(3) 0.0265(8) Uani 1 1 d . . .
O12 O -0.6283(3) -0.3929(3) -0.3259(3) 0.0150(6) Uani 1 1 d . . .
O13 O -0.7490(3) -0.4218(3) -0.5616(3) 0.0149(7) Uani 1 1 d . . .
O14 O -0.9356(3) -0.1939(3) -0.3940(3) 0.0161(7) Uani 1 1 d . . .
C1 C -0.3729(5) -0.0734(4) 0.3344(4) 0.0233(11) Uani 1 1 d . . .
H1 H -0.2918 -0.0040 0.3594 0.028 Uiso 1 1 calc R . .
C2 C -0.4356(6) -0.1652(5) 0.0366(5) 0.0346(13) Uani 1 1 d . . .
H2A H -0.5082 -0.2455 0.0113 0.041 Uiso 1 1 calc R . .
H2B H -0.4383 -0.1360 -0.0352 0.041 Uiso 1 1 calc R . .
C3 C -0.4709(6) -0.0833(5) 0.1108(5) 0.0286(12) Uani 1 1 d . . .
H3A H -0.4022 -0.0017 0.1317 0.034 Uiso 1 1 calc R . .
H3B H -0.5646 -0.0823 0.0630 0.034 Uiso 1 1 calc R . .
C4 C -0.5729(5) -0.2220(4) 0.2174(4) 0.0151(9) Uani 1 1 d U . .
H4 H -0.6525 -0.2739 0.1503 0.018 Uiso 1 1 calc R . .
C5 C -0.2548(8) -0.2535(7) 0.0287(6) 0.0468(17) Uani 1 1 d . . .
H5A H -0.1726 -0.2688 0.0817 0.056 Uiso 1 1 calc R . .
H5B H -0.3338 -0.3303 -0.0082 0.056 Uiso 1 1 calc R . .
C6 C -0.0874(5) -0.1435(5) -0.0492(4) 0.0277(12) Uani 1 1 d U . .
H6 H -0.0045 -0.1288 0.0196 0.033 Uiso 1 1 calc R . .
C7 C -0.2926(7) -0.1734(7) 0.1021(5) 0.0461(16) Uani 1 1 d . . .
H7A H -0.2906 -0.2036 0.1733 0.055 Uiso 1 1 calc R . .
H7B H -0.2204 -0.0929 0.1286 0.055 Uiso 1 1 calc R . .
C8 C -0.3090(6) -0.2047(5) -0.1754(5) 0.0288(12) Uani 1 1 d . . .
H8 H -0.4079 -0.2408 -0.2073 0.035 Uiso 1 1 calc R . .
N1 N -0.5346(6) -0.2292(5) 0.3300(4) 0.0400(12) Uani 1 1 d U . .
N2 N -0.0994(6) -0.1124(6) -0.1523(5) 0.0513(14) Uani 1 1 d U . .
N3 N -0.2222(5) -0.2010(4) -0.0669(4) 0.0293(10) Uani 1 1 d U . .
N4 N -0.2357(4) -0.1492(4) -0.2344(3) 0.0217(9) Uani 1 1 d U . .
N5 N -0.4695(5) -0.1215(4) 0.2216(4) 0.0242(9) Uani 1 1 d U . .
N6 N -0.4107(4) -0.1404(4) 0.4060(3) 0.0205(9) Uani 1 1 d U . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N6 Zn1 N4 168.54(16) 1_554 .
N6 Zn1 O6W 93.21(15) 1_554 .
N4 Zn1 O6W 91.99(15) . .
N6 Zn1 O7W 97.27(16) 1_554 .
N4 Zn1 O7W 92.99(16) . .
O6W Zn1 O7W 89.40(14) . .
N6 Zn1 O8W 85.77(15) 1_554 .
N4 Zn1 O8W 88.51(15) . .
O6W Zn1 O8W 176.97(14) . .
O7W Zn1 O8W 93.56(14) . .
N6 Zn1 O10 85.85(14) 1_554 .
N4 Zn1 O10 83.89(14) . .
O6W Zn1 O10 90.66(13) . .
O7W Zn1 O10 176.88(14) . .
O8W Zn1 O10 86.43(13) . .
O1W Zn2 O1W 180.0(2) . 2_545
O1W Zn2 O2W 91.60(18) . 2_545
O1W Zn2 O2W 88.40(18) 2_545 2_545
O1W Zn2 O2W 88.40(18) . .
O1W Zn2 O2W 91.60(18) 2_545 .
O2W Zn2 O2W 180.0 2_545 .
O1W Zn2 O5W 89.91(18) . 2_545
O1W Zn2 O5W 90.09(18) 2_545 2_545
O2W Zn2 O5W 89.32(17) 2_545 2_545
O2W Zn2 O5W 90.68(17) . 2_545
O1W Zn2 O5W 90.09(18) . .
O1W Zn2 O5W 89.91(18) 2_545 .
O2W Zn2 O5W 90.68(17) 2_545 .
O2W Zn2 O5W 89.32(17) . .
O5W Zn2 O5W 180.00(19) 2_545 .
O13 V1 O7 106.10(15) . .
O13 V1 O8 98.61(14) . .
O7 V1 O8 95.66(15) . .
O13 V1 O5 98.05(15) . .
O7 V1 O5 96.04(14) . .
O8 V1 O5 156.10(13) . .
O13 V1 O4 89.08(14) . .
O7 V1 O4 164.82(14) . .
O8 V1 O4 82.07(13) . .
O5 V1 O4 81.19(12) . .
O13 V1 O4 167.95(13) . 2_344
O7 V1 O4 85.95(13) . 2_344
O8 V1 O4 79.97(12) . 2_344
O5 V1 O4 80.15(12) . 2_344
O4 V1 O4 78.88(12) . 2_344
O13 V1 V3 41.09(11) . .
O7 V1 V3 147.19(11) . .
O8 V1 V3 91.13(10) . .
O5 V1 V3 90.25(10) . .
O4 V1 V3 47.99(8) . .
O4 V1 V3 126.86(8) 2_344 .
O13 V1 V2 142.92(11) . 2_344
O7 V1 V2 36.82(10) . 2_344
O8 V1 V2 88.71(10) . 2_344
O5 V1 V2 88.26(10) . 2_344
O4 V1 V2 128.00(9) . 2_344
O4 V1 V2 49.13(8) 2_344 2_344
V3 V1 V2 175.93(3) . 2_344
O11 V2 O2 104.09(16) . .
O11 V2 O1 101.96(17) . .
O2 V2 O1 91.03(14) . .
O11 V2 O14 102.88(17) . .
O2 V2 O14 89.45(14) . .
O1 V2 O14 154.25(14) . .
O11 V2 O7 100.57(16) . 2_344
O2 V2 O7 155.33(13) . 2_344
O1 V2 O7 84.44(14) . 2_344
O14 V2 O7 84.45(14) . 2_344
O11 V2 O4 175.71(15) . .
O2 V2 O4 80.20(12) . .
O1 V2 O4 77.69(12) . .
O14 V2 O4 77.04(12) . .
O7 V2 O4 75.14(11) 2_344 .
O11 V2 V3 136.84(13) . .
O2 V2 V3 32.75(9) . .
O1 V2 V3 84.06(10) . .
O14 V2 V3 82.50(10) . .
O7 V2 V3 122.59(9) 2_344 .
O4 V2 V3 47.44(7) . .
O11 V2 V1 131.46(13) . 2_344
O2 V2 V1 124.45(10) . 2_344
O1 V2 V1 79.09(10) . 2_344
O14 V2 V1 79.46(10) . 2_344
O7 V2 V1 30.89(9) 2_344 2_344
O4 V2 V1 44.26(7) . 2_344
V3 V2 V1 91.70(4) . 2_344
O10 V3 O2 104.70(16) . .
O10 V3 O9 101.98(15) . .
O2 V3 O9 93.32(15) . .
O10 V3 O12 100.13(16) . .
O2 V3 O12 92.08(15) . .
O9 V3 O12 155.08(14) . .
O10 V3 O13 97.52(15) . .
O2 V3 O13 157.75(13) . .
O9 V3 O13 83.16(13) . .
O12 V3 O13 82.67(14) . .
O10 V3 O4 171.82(14) . .
O2 V3 O4 83.38(12) . .
O9 V3 O4 78.48(12) . .
O12 V3 O4 78.01(12) . .
O13 V3 O4 74.38(11) . .
O10 V3 V1 129.20(12) . .
O2 V3 V1 126.07(10) . .
O9 V3 V1 78.93(10) . .
O12 V3 V1 78.24(10) . .
O13 V3 V1 31.69(8) . .
O4 V3 V1 42.69(8) . .
O10 V3 V2 138.45(12) . .
O2 V3 V2 33.77(10) . .
O9 V3 V2 86.13(10) . .
O12 V3 V2 84.93(10) . .
O13 V3 V2 123.99(9) . .
O4 V3 V2 49.62(8) . .
V1 V3 V2 92.30(4) . .
O10 V3 V4 134.50(12) . .
O2 V3 V4 83.00(10) . .
O9 V3 V4 32.56(9) . .
O12 V3 V4 124.70(10) . .
O13 V3 V4 82.34(9) . .
O4 V3 V4 46.70(8) . .
V1 V3 V4 62.13(3) . .
V2 V3 V4 61.49(4) . .
O10 V3 V5 131.94(12) . .
O2 V3 V5 82.59(11) . .
O9 V3 V5 125.31(10) . .
O12 V3 V5 31.84(9) . .
O13 V3 V5 81.63(9) . .
O4 V3 V5 46.84(7) . .
V1 V3 V5 61.57(4) . .
V2 V3 V5 61.21(3) . .
V4 V3 V5 93.28(3) . .
O6 V4 O14 103.13(16) . .
O6 V4 O9 101.95(16) . .
O14 V4 O9 94.56(14) . .
O6 V4 O8 101.77(15) . 2_344
O14 V4 O8 89.86(14) . 2_344
O9 V4 O8 154.18(13) . 2_344
O6 V4 O5 101.03(16) . .
O14 V4 O5 153.98(13) . .
O9 V4 O5 89.76(13) . .
O8 V4 O5 75.82(12) 2_344 .
O6 V4 O4 175.84(15) . .
O14 V4 O4 80.53(12) . .
O9 V4 O4 79.56(12) . .
O8 V4 O4 76.10(12) 2_344 .
O5 V4 O4 75.04(12) . .
O6 V4 V5 91.11(12) . 2_344
O14 V4 V5 129.62(10) . 2_344
O9 V4 V5 129.73(10) . 2_344
O8 V4 V5 39.76(9) 2_344 2_344
O5 V4 V5 39.97(9) . 2_344
O4 V4 V5 84.99(8) . 2_344
O6 V4 V3 135.06(13) . .
O14 V4 V3 82.19(10) . .
O9 V4 V3 33.45(10) . .
O8 V4 V3 123.02(9) 2_344 .
O5 V4 V3 87.55(9) . .
O4 V4 V3 46.91(7) . .
V5 V4 V3 120.00(4) 2_344 .
O3 V5 O12 103.50(17) . .
O3 V5 O1 103.10(17) . .
O12 V5 O1 94.90(14) . .
O3 V5 O8 101.25(16) . .
O12 V5 O8 90.37(14) . .
O1 V5 O8 153.10(13) . .
O3 V5 O5 101.02(16) . 2_344
O12 V5 O5 153.81(13) . 2_344
O1 V5 O5 88.35(13) . 2_344
O8 V5 O5 75.88(12) . 2_344
O3 V5 O4 175.75(15) . .
O12 V5 O4 79.18(12) . .
O1 V5 O4 79.81(12) . .
O8 V5 O4 75.31(12) . .
O5 V5 O4 75.84(11) 2_344 .
O3 V5 V4 90.77(13) . 2_344
O12 V5 V4 130.15(11) . 2_344
O1 V5 V4 128.36(10) . 2_344
O8 V5 V4 39.79(9) . 2_344
O5 V5 V4 40.01(8) 2_344 2_344
O4 V5 V4 84.99(8) . 2_344
O3 V5 V3 136.58(13) . .
O12 V5 V3 33.40(10) . .
O1 V5 V3 82.45(10) . .
O8 V5 V3 87.71(9) . .
O5 V5 V3 122.31(9) 2_344 .
O4 V5 V3 46.47(8) . .
V4 V5 V3 119.72(4) 2_344 .
V5 O1 V2 115.95(16) . .
V3 O2 V2 113.48(16) . .
V1 O4 V1 101.12(12) . 2_344
V1 O4 V4 94.22(12) . .
V1 O4 V4 92.75(11) 2_344 .
V1 O4 V3 89.32(11) . .
V1 O4 V3 169.55(15) 2_344 .
V4 O4 V3 86.39(10) . .
V1 O4 V5 93.05(11) . .
V1 O4 V5 92.71(11) 2_344 .
V4 O4 V5 169.90(15) . .
V3 O4 V5 86.69(10) . .
V1 O4 V2 172.22(15) . .
V1 O4 V2 86.62(10) 2_344 .
V4 O4 V2 86.18(10) . .
V3 O4 V2 82.94(10) . .
V5 O4 V2 85.68(10) . .
V1 O5 V4 106.74(14) . .
V1 O5 V5 108.96(14) . 2_344
V4 O5 V5 100.01(13) . 2_344
V1 O7 V2 112.29(16) . 2_344
V1 O8 V5 106.69(14) . .
V1 O8 V4 108.74(14) . 2_344
V5 O8 V4 100.45(14) . 2_344
V4 O9 V3 113.99(16) . .
V3 O10 Zn1 173.3(2) . .
V5 O12 V3 114.75(16) . .
V1 O13 V3 107.22(15) . .
V4 O14 V2 115.69(16) . .
N5 C1 N6 109.2(4) . .
C7 C2 C3 113.5(5) . .
N5 C3 C2 112.4(4) . .
N1 C4 N5 103.7(4) . .
N3 C5 C7 113.3(5) . .
N2 C6 N3 103.7(4) . .
C2 C7 C5 114.2(5) . .
N3 C8 N4 110.3(5) . .
C4 N1 N6 113.5(5) . .
C6 N2 N4 113.0(5) . .
C8 N3 C6 110.2(4) . .
C8 N3 C5 129.2(5) . .
C6 N3 C5 120.6(5) . .
C8 N4 N2 102.8(4) . .
C8 N4 Zn1 130.6(3) . .
N2 N4 Zn1 126.5(4) . .
C1 N5 C4 109.9(4) . .
C1 N5 C3 129.2(4) . .
C4 N5 C3 120.9(4) . .
C1 N6 N1 103.8(4) . .
C1 N6 Zn1 131.1(3) . 1_556
N1 N6 Zn1 124.9(3) . 1_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zn1 N6 2.069(4) 1_554
Zn1 N4 2.086(4) .
Zn1 O6W 2.088(3) .
Zn1 O7W 2.117(4) .
Zn1 O8W 2.180(4) .
Zn1 O10 2.222(3) .
Zn2 O1W 2.067(4) .
Zn2 O1W 2.067(4) 2_545
Zn2 O2W 2.072(4) 2_545
Zn2 O2W 2.072(4) .
Zn2 O5W 2.158(4) 2_545
Zn2 O5W 2.158(4) .
V1 O13 1.675(3) .
V1 O7 1.715(3) .
V1 O8 1.928(3) .
V1 O5 1.936(3) .
V1 O4 2.066(3) .
V1 O4 2.160(3) 2_344
V1 V3 3.0463(13) .
V1 V2 3.0901(13) 2_344
V2 O11 1.606(3) .
V2 O2 1.848(3) .
V2 O1 1.863(3) .
V2 O14 1.886(3) .
V2 O7 2.002(3) 2_344
V2 O4 2.341(3) .
V2 V3 3.0496(14) .
V2 V1 3.0901(13) 2_344
V3 O10 1.616(3) .
V3 O2 1.799(3) .
V3 O9 1.866(3) .
V3 O12 1.889(3) .
V3 O13 2.096(3) .
V3 O4 2.264(3) .
V3 V4 3.0932(17) .
V3 V5 3.1168(14) .
V4 O6 1.614(3) .
V4 O14 1.823(3) .
V4 O9 1.822(3) .
V4 O8 2.005(3) 2_344
V4 O5 2.012(3) .
V4 O4 2.256(3) .
V4 V5 3.0808(13) 2_344
V5 O3 1.594(3) .
V5 O12 1.811(3) .
V5 O1 1.841(3) .
V5 O8 2.004(3) .
V5 O5 2.010(3) 2_344
V5 O4 2.277(3) .
V5 V4 3.0808(13) 2_344
O4 V1 2.160(3) 2_344
O5 V5 2.010(3) 2_344
O7 V2 2.002(3) 2_344
O8 V4 2.005(3) 2_344
C1 N5 1.328(6) .
C1 N6 1.331(6) .
C2 C7 1.494(8) .
C2 C3 1.506(7) .
C3 N5 1.470(6) .
C4 N1 1.307(6) .
C4 N5 1.351(6) .
C5 N3 1.483(7) .
C5 C7 1.504(9) .
C6 N2 1.323(7) .
C6 N3 1.334(7) .
C8 N3 1.301(7) .
C8 N4 1.338(7) .
N1 N6 1.353(6) .
N2 N4 1.346(7) .
N6 Zn1 2.069(4) 1_556
